RAP or RAS? The Differences in Performance of HMA Containing Reclaimed Asphalt Pavement and Reclaimed Asphalt Shingles JENNIFER J. FOXLOW1, JO SIAS DANIEL2, and ARAVIND KRISHNA SWAMY3 The use of Reclaimed Asphalt Pavement (RAP) in Hot Mix Asphalt (HMA) has become a widely accepted practice by most of the paving industry. As the cost of virgin materials continue to rise, the use of cost efficient and quality recycled materials is also increasing, and Reclaimed Asphalt Shingles (RAS) have begun to be considered a viable source of recycled binder and aggregate. This study compares the laboratory performance of four HMA mixes: one that contains only RAP, and three mixes that contain different RAS products. Superpave mixture designs resulted in higher asphalt contents and VMA values for the RAS mixtures as compared to the RAP mixture. Testing included the determination of PG grade, shear modulus and phase angle, creep stiffness and slope values, and critical cracking temperatures for binder recovered from the HMA mixtures. Mixture testing included complex modulus and Thermal Stress Restrained Specimen Tensile Strength tests on all four mixtures and fatigue testing on two mixtures. The Hirsch model was used to back calculate the binder shear modulus; values for binder modulus and phase angle were used to determine the effective high temperature PG grade of the mixtures. The binder testing indicates that the RAS mixtures are stiffer than the RAP mix at high temperatures and would perform better with respect to low temperature cracking. The mixture testing shows that the RAP mix is stiffer and has a poorer fatigue resistance at intermediate temperatures than the RAS mixtures, while all four mixtures have similar low temperature performance. KEY WORDS: Reclaimed Asphalt Pavement, Reclaimed Asphalt Shingles, Binder Testing, Low Temperature and Fatigue Testing 1 Research Assistant, Masters candidate, 2PhD, P.E., Associate Professor of Civil Engineering and Research Assistant, PhD candidate, Civil Engineering Department, University of New Hampshire, Durham, NH 3 INTRODUCTION The use of recycled materials in the form of Reclaimed Asphalt Pavement (RAP) and Reclaimed Asphalt Shingles (RAS) in Hot Mix Asphalt (HMA) has become regular practice for much of the country. As an alternative supply of both quality aggregate and asphalt, the use of RAP and RAS effectively cuts the cost of HMA production, and as the cost of virgin materials continue to rise, much of the paving industry has begun to look more seriously at increasing the use of these materials. RAP is generated when the materials from pavements are milled and crushed. RAS is generated from scrap shingle materials that can come from either factory waste or post-consumer (tear-offs) waste. Because of the difference in origins of these materials, and the fact that RAP contains paving grade asphalt while RAS does not, the properties of these materials can be very different, and may produce different effects when introduced to an HMA mixture. The addition of these recycled materials to an asphalt mixture changes the mechanistic properties (i.e., strength) of the mixture and affects its performance (i.e., resistance to cracking and deformation) in the field. This is a result of the aged binder being introduced to the mixture as a part of the RAP and RAS, as this binder has a different chemical composition and different properties than the virgin binder being added to the mix (1). Previous studies on RAP (2-8) have shown that the virgin and recycled binders will mix to some extent, which will change the properties of the mixture containing RAP when compared to one that contains only virgin material. The extent of this blending is unknown and may be different for the various RAP and RAS sources and virgin binders. The actual, or effective, properties of the binder in mixtures containing RAP and/or RAS cannot be tested directly, as the process of extracting the binder for testing results in complete blending of the virgin and RAP binder; therefore, testing must be performed on the mixtures to determine the effective binder properties (1). Currently, RAS to be used in HMA is generally shredded or ground to a 3/8” maximum nominal size product. An alternative processing method exists in which the shingles are first cleaned of non-aggregate material (i.e., wood chips, roofing nails, tape) that is common in stockpiles of both the factory tearoff and the post-consumer scrap. The shingles are then ground to a maximum nominal size of a #16 sieve size, which is subsequently separated into an above #50 (+50) mesh and a below #50 (-50) mesh stockpile. By separating the two gradations, the +50 mesh product has reduced fines content, making it ideal for use as a recycled aggregate in HMA mixtures, while the -50 mesh shingles can be used in other applications. Research Objective The objective of this research study was to evaluate the behavior and performance of three different RAS products with respect to a control mixture containing RAP only. The differences in the mixtures are evaluated with respect to mix design volumetrics, complex modulus, low temperature testing, and fatigue testing. Binder testing was also performed on the source materials and extracted material from each mixture. MATERIALS AND TESTING METHODS Materials Virgin Aggregates Virgin aggregates used in this project were donated from Pike Industries, Inc. and obtained from their Portsmouth, NH plant. The 12.5 mm, 9.5 mm and primary dust stockpiles came from Pike’s Eliot, ME quarry, while the washed sand and washed manufactured sand came from the Madbury, NH quarry. Virgin Asphalt Binder Virgin asphalt binder used in this project was donated from Pike Industries and obtained from their Portsmouth, NH plant. The binder was a PG 64 – 28, and contained a PPA (polyphosphoric acid) modifier. The mixing temperature was 165 °C and the compaction temperature was 145 °C. The continuous grade of the virgin binder is shown in Table 1. Reclaimed Asphalt Pavement (RAP) The RAP used in this project was donated from Pike Industries and obtained from their Portsmouth, NH plant. The extracted PG grade of the RAP binder was 88 – 22. The actual and continuous PG grade of the RAP binder is shown in Table 1. The asphalt content and gradation of the RAP stockpile is shown in Table 2. Dynamic Shear values for the recovered binder before and after Rolling Thin Film Oven (RTFO) test are shown in Tables 3 and 4, respectively. The creep stiffness (S) and slope (m) results obtained from the bending beam rheometer test are shown in Table 5. Reclaimed Asphalt Shingles (RAS) Three sources of post-consumer RAS were used in this project. The normally ground shingles were donated from ERRCO in Epping, NH. RASTech Inc. in Brentwood, NH provided the separated +50 mesh and -50 mesh shingles. The asphalt contents as well as the gradations of the shingles were measured and are shown in Table 2. The recovered binder from the RAS was too stiff to grade using available equipment, although it should be noted that it is possible that fibers from the RAS materials could have still been present in the binder, which could affect the recovered binder properties. Dynamic shear values for the recovered RAS binders before and after RTFO aging are shown in Tables 3 and 4, respectively, and creep stiffness and slope values are presented in Table 5. The binder from the normal ground shingles is the stiffest and least compliant while the other two RAS binder types are similar, which is expected because they are derived from the same shingles source. Table 1: Asphalt Grades from Each Source of Binder Source PG Grade Continuous PG Grade 88 – 22 89.3 – 22.0 Normal Ground Shingles n/a* n/a* +50 Mesh Shingles -50 Mesh Shingles n/a* n/a* n/a* n/a* 64 – 28 65.1 – 29.8 RAP Virgin Binder * PG grade could not be measured Table 2: RAP and RAS Aggregate Gradation and Asphalt Content % Passing Sieve size RAP Normal Ground +50 Mesh -50 Mesh 12.5 (1/2”) 9.5 (3.8”) 4.75 (#4) 2.36 (#8) 1.18 (#16) 0.6 (#30) 0.3 (#50) 0.15 (#100) 0.075 (#200) % ac 100 98 75 58 46 34 22 13 7.6 4.37% 100 100 97.0 94.3 67.5 42.6 36.2 30.2 23.6 23.62% 100 100 100 100 77.1 39.1 26.8 21.2 17.4 12.1% Table 3: G*/sin δ Values for Recovered Binder Source Temperature G*/sinδ (°C) (kPa) RAP 88 1.17 94 0.94 Normal Ground Shingles 112 151.8 118 89.90 +50 Mesh Shingles 112 15.49 118 8.28 -50 Mesh Shingles 112 8.85 118 5.43 100 100 100 100 100 94.1 90.3 74.3 57.5 28.0% Table 4: G*/sin δ Values for Rolling Thin Film Oven Residue Source Temperature G*/sinδ Temperature G*sinδ (°C) (kPa) (°C) (kPa) RAP 88 2.53 28 °C 4098 94 1.33 25 °C 5696 Normal Ground 112 171.03 37 °C 4681 Shingles 118 99.82 34 °C 5268 +50 Mesh 112 31.56 28 °C 4990 Shingles 118 20.95 25 °C 5903 -50 Mesh 112 19.96 25 °C 4930 Shingles 118 12.66 22 °C 5846 Table 5: Creep Stiffness and Slope Values at 60 s for Recovered Binder S Temperature m-value Source (MPa) (°C) RAP -12 -18 0 -30 218 419 109 690 0.300 0.240 0.206 0.155 +50 Mesh Shingles 0 -30 62 612 0.266 0.177 -50 Mesh Shingles 0 -30 32.6 655 0.277 0.177 Normal Ground Shingles Mix Design Mix designs using an NHDOT Type E, 12.5 mm (1/2”) Superpave Surface Course mix design as a template were performed in this project. The same target gradation was used for each mixture to allow a more direct evaluation of the different RAP/RAS contents on the material properties. The mixtures were designed for light traffic (less than 0.3 million ESALs) using a gyratory compactive effort of Ndes=50. The 2009 NHDOT specifications (9) permit recycled binder in mix designs of up to 0.8%, 0.6% of which can come from shingles, without requiring binder bumping or additional testing. Each mixture in this study contains 0.8% recycled binder; the RAS mixtures contain the maximum 0.6% with the additional 0.2% coming from RAP. The gradations and design asphalt contents for each mixture are shown in Table 6, and the volumetrics for the four mixtures are shown in Table 7. The shingles mixtures require more virgin binder than the RAP only mixture, with the normal ground shingle mix requiring the most. The VMAs of the RAS mixtures are higher than the RAP only mixture, with the ground shingles mixture being the highest. The VFA of the ground shingles mixture is higher than the RAP only mixture while the +50 mesh and -50 mesh mixtures have lower VFA values. Table 6: Mixture Gradations, Asphalt Contents % Passing RAP Mix with Mix with Mix with Sieve size Only Normal Ground +50 Mesh -50 Mesh Mix Shingles Shingles Shingles 19.0 (3/4”) 100.0 100.0 100.0 100.0 12.5 (1/2”) 98.7 98.7 98.7 98.7 9.5 (3.8”) 86.0 86.0 86.0 86.0 4.75 (#4) 57.9 57.9 57.9 57.9 2.36 (#8) 43.0 43.0 43.0 43.0 1.18 (#16) 32.4 32.4 32.4 32.4 0.6 (#30) 22.6 22.6 22.6 22.6 0.3 (#50) 13.2 13.2 13.2 13.2 0.15 (#100) 5.8 5.8 5.8 5.8 0.075 (#200) 3.2 3.2 3.2 3.2 RAP ac 0.8% 0.2% 0.2% 0.2% RAS ac 0.0% 0.6% 0.6% 0.6% 4.9% 5.7% 5.2% 5.3% Virgin ac Total ac 5.7% 6.5% 6.0% 6.1% % Recycled Binder 14.0% 12.3% 13.3% 13.1% Table 7: Mixture Volumetrics Voids-in-the Voids Filled With Mineral Aggregate Asphalt (VFA, %) (VMA, %) Superpave Criteria ≥ 14.0 70 – 80 RAP Only Mix 15.8 76.9 Mix with Normal Ground Shingles Mix with +50 Mesh Shingles Mix with -50 Mesh Shingles 17.2 77.0 16.1 75.7 16.6 75.4 Specimen Fabrication All virgin aggregate was sieved and stored in separate 5 gallon buckets by sieve size. The RAP and RAS were stored as individual stockpiles, unsieved. Virgin aggregate for each specimen was batched by individual sieve size, while the RAP and RAS were batched as a stockpile, assuming that a representative sample was taken from each stockpile. Virgin aggregates, RAP, and RAS were cold blended prior to any heating to aid in mixing. If preblending was not done, agglomerations of the materials would occur due to their high asphalt contents. These mixtures were heated along with the virgin binder for the period of time required for the asphalt to come to proper mixing temperature (165 °C), generally 1.5 to 2 hours. Once combined in a bucket mixer, the HMA was short term aged for two hours at the compaction temperature. The specimens were then compacted to a specified height using a Superpave Gyratory Compactor (SGC). After compaction, the specimens were allowed to cool to room temperature overnight, and cored and cut using to testing dimensions (75 mm diameter, 150 mm height). The Gmb of all specimens were measured using a Corelok Vacuum Sealing system. The air void content, VMA, and VFA values were calculated for each specimen. The bulk specific gravity (Gsb) of the shingles aggregate was not directly measured; instead, a range of possible VMA and VFAs were calculated for each specimen based on typical Gsb values of the aggregates in shingles. The analysis determined that the range of Gsb values did not have a large enough impact on the VMA and VFA of a specimen to be considered significant; therefore, the average value of Gsb was used. All specimens used in this study fell within the target air void range of 4%, ± 0.5%. Testing Setup and Equipment The complex modulus, low temperature and, fatigue tests performed in this study were conducted using a closed-loop servo-hydraulic system, manufactured by Instron®. The testing apparatus includes the loading frame (model 8800), a 20k kip hydraulic load actuator (model IST 3690 Series 100kN Pedestal Mounted Actuator), a 5 kip load cell, a 20 kip load cell, control tower (model 8500), a control panel (model 8500 Plus), an environmental chamber (model 3119-407), and personal computers running Instron’s Fast Track 2 Software (actuator control), Labview 7.1 (data acquisition), Microsoft® Excel and MATLAB (data and statistical analysis) (1). The set up for the low temperature test also required a National Instruments Hi-Speed USB Carrier (NI USB-9162). An Envirotherm® environmental chamber was used to set the testing environment desired using low pressure nitrogen. The chamber controlled the temperature within ±0.1 °C with a Eurotherm® thermostat (model 2408); the testing was performed between -20 and 20 °C. During testing, a dummy sample of the same dimensions of the test specimens with a thermocouple permanently inserted was placed within the environmental chamber in order to monitor the internal temperature of the test specimen. Specimen Preparation Specimens were prepped for complex modulus and the Thermal Stress Restrained Specimen Tensile Strength Test (TSRST) simultaneously. Metal end plates were attached to the specimens and the epoxy was allowed to cure a minimum of 12 hours. In order to measure the uniaxial strain placed on the specimen during complex modulus testing, four Linearly Variable Differential Transducers (LVDTs) were attached to the specimen using L-shaped brackets that were attached with screws to brass targets that had been set with epoxy on the specimen. Each LVDT had a gage length of 100 mm along the vertical axis of the specimen, and the four LVDTs were oriented 90° from each other around the specimen. A separate set of specimens were prepared for fatigue testing and were instrumented similarly. Once complex modulus testing was completed for each specimen, it was prepped for a TSRST test. The specimen remained in the environmental chamber (unrestrained) and was allowed to cool to the starting test temperature of -5 °C. LVDTs were removed from the surface and replaced with three thermocouples connected to the NI hi-speed USB carrier at the top, middle and bottom of the specimen to measure surface temperature. These thermocouples were held in place with clay putty. Binder Modulus and Binder Phase Angle Testing Asphalt binder was extracted and recovered from cores of each of the four HMA mixtures. The binder modulus and phase angle for the recovered binders and for the virgin binder were measured over a range of 0.10 to 100.00 Hz at 10, 22, 34 and 46 °C. The individual isotherms were shifted to the reference temperature of 20 °C and fitted with generalized logistic function. The generalized logistic function form used with shear modulus is presented in Equation 1. log|𝐺 ∗ | = 𝑎 + 𝑏 [1+𝑒∙𝑒𝑥𝑝𝑐+𝑑(log 𝜔𝑟) ] (1/𝑒) (1) where: |G*| = Shear Modulus ωr = reduced angular frequency a, b, c, d, e = regression coefficients The binder phase angle master curves were also shifted to the reference temperature of 20 °C, and subsequently fitted with the differential form of the generalized logistic function modified to suit phase angle: 𝛿𝑏 = −90 × 𝑏𝑑 𝑒 𝑐+𝑑(𝑙𝑜𝑔𝜔𝑟) (1+1/𝑒) (1+𝑒∙𝑒𝑥𝑝𝑐+𝑑(𝑙𝑜𝑔𝜔𝑟) ) where: δb = Phase Angle ωr = reduced angular frequency (2) b, c, d, e = regression coefficients Complex Modulus Testing Complex modulus testing was performed in uniaxial tension mode. The dynamic modulus, |E*|, was calculated using the equation: |𝐸 ∗ | = 𝜎𝑎𝑚𝑝 (3) 𝜀𝑎𝑚𝑝 Where σamp is the amplitude of the applied stress waveform and εamp is the amplitude of the strain response. Testing was completed at frequencies of 0.1, 0.2, 0.5, 1, 2, 5, 10 and 20 Hz and at temperatures of 20, 10, 0, -10 and -20 °C. The dynamic modulus master curves for each individual specimen (three replicates tested for each mixture) were constructed at a reference temperature of 20°C, and then fitted with a standard logistic function: log|𝐸 ∗ | = 𝑎 + 𝑏 (4) 1+𝑒𝑥𝑝𝑐+𝑑(log 𝜔𝑟) where: |E*| = Dynamic Modulus ωr = reduced angular frequency a, b, c, d = regression coefficients The dynamic modulus master curve of a mixture was then determined by fitting an average curve to all the specimen master curves for that mix. The phase angle master curve was developed in the same fashion, using the same shift factors used to develop the corresponding |E*| master curve. Equation 5 shows standard logistic function used for the phase angle curves: 𝛿 = −90 × 𝑏𝑑 𝑒𝑥𝑝𝑐+𝑑(𝑙𝑜𝑔𝜔𝑟) 2 (1+𝑒𝑥𝑝𝑐+𝑑(𝑙𝑜𝑔𝜔𝑟) ) (5) where: δ = Phase Angle ωr = reduced angular frequency b, c, d = regression coefficients Hirsch Model In this project, the Hirsch model was used to forward calculate the dynamic modulus from the binder modulus, |G*|, as measured on the extracted mix binders as well as the virgin binder. Originally developed in the late 1960’s by T.J. Hirsch, this model was used to calculate the modulus of elasticity of concrete. In 2003, Christensen, Pellinen, and Bonaquist (10) refined this model to predict the dynamic modulus of HMA using the binder modulus and volumetrics of the mix. This version of the Hirsch modulus follows the equation: |𝐸 ∗ |𝑚𝑖𝑥 = 𝑃𝑐 ∙ [4,200,000 ∙ (1 − 𝑉𝑀𝐴 𝑉𝐹𝐴 ∙ 𝑉𝑀𝐴 ) + 3 ∙ |𝐺 ∗ |𝑏𝑖𝑛𝑑𝑒𝑟 ∙ ( )] + 100 10,000 (1 − 𝑃𝑐) ∙ [ 𝑃𝑐 = 𝑉𝑀𝐴 100 1− 4,200,000 −1 + 𝑉𝑀𝐴 3∙𝑉𝐹𝐴∙|𝐺 ∗ |𝑏𝑖𝑛𝑑𝑒𝑟 0.58 𝑉𝐹𝐴∙3∙|𝐺∗ |𝑏𝑖𝑛𝑑𝑒𝑟 ) 𝑉𝑀𝐴 𝑉𝐹𝐴∙3∙|𝐺∗ |𝑏𝑖𝑛𝑑𝑒𝑟 0.58 650+( ) 𝑉𝑀𝐴 ] (6) (20+ (7) Where: VMA = Voids in mineral aggregate VFA = Voids filled with asphalt Pc = Contact area It should be noted that the Hirsh model requires English units, and dynamic modulus values must be converted from MPa to psi before using this model. Binder shear modulus (|𝐺 ∗ |𝑏𝑖𝑛𝑑𝑒𝑟 ) was back calculated through Hirsch model using individual specimen volumetrics and |𝐸 ∗ | values. The |E*| master curve for a mix was constructed using its respective logistic function coefficients over the range of 0.1 – 4000 Hz at regular intervals. Using equations 6 and 7, the |G*|binder values at these individual frequencies were found by minimizing error between measured |E*| (averaged through regression coefficients) and predicted |E*| from Hirsch model. These back calculated |G*|binder values were subsequently fit using the ChristiansenAnderson model (11), λ 𝛽 −1/𝛽 |𝐺 ∗ | = 𝐺0 [1 + ( ) ] 𝜔𝑟 (8) Where: G0 = Glassy Modulus ωr = reduced angular frequency λ, β = regression coefficients. Effective PG Determination To determine the effective performance grade of each mixture, the binder shear modulus and phase angle master curves were first shifted to different temperatures using appropriate shift factors. The log of the shift factors for the binder and dynamic modulus data were fitted with a second order polynomial equation. Due to the limited range of testing temperatures, shift factors at the higher temperatures were extrapolated using the fitted polynomial equation. The effective high temperature PG grade of the binder in the mix is determined as the temperature that corresponds with the value of |G*|/sin(δ) = 2.2 kPa at 1.6 Hz. The values for |G*| were determined by shifting the binder modulus master curve to the appropriate temperature and then determining the |G*| value at 1.6 Hz for that temperature. The same procedure was used to determine the δ at those test temperatures. The |G*|/sin(δ) values were calculated and plotted against temperature. In this study, both the measured values of the binder shear modulus from the extracted (fully blended) mix binder and the back-calculated binder shear modulus using the Hirsch model were used to determine the effective PG grade. Thermal Stress Restrained Specimen Tensile Strength (TSRST) Test The TSRST test was performed to assess the low temperature performance of each of the four HMA mixes. The test followed AASHTO procedure TP 10-93, with modified testing apparatus and specimen dimensions, as well as initial temperature of the test (12). In this study, the test began once the specimen reached an internal temperature of -5 °C, as measured by the internal temperature of a dummy specimen placed in the environmental chamber at the same time as the test sample. Once the target temperature was reached, the specimen was restrained by screwing the end plates of the specimen into place on the uniaxial testing jig. The specimen was then cooled at a rate of -6 °C per hour. The thermally induced load was measured with a load cell and recorded using LabView until fracture of the specimen occurred. The temperature as well as the load measured from the Instron at the point of fracture was noted. Fatigue Testing Fatigue testing was conducted on the RAP mixture and the mixture with +50 mesh shingles according to proposed standard for determining the damage characteristic curve of asphalt concrete from direct tension cyclic fatigue tests (13). The test specimens were instrumented with end plates and LVDT’s and placed in an environmental chamber at 20 °C until equilibrium was reached. The specimen was fixed in the loading frame and the dynamic modulus was determined. Once the |𝐸 ∗ | fingerprint was obtained, the specimen was tested in fatigue using a loading frequency of 10Hz. The strain amplitude was adjusted so that the specimens were expected to fail at around 1000 cycles or 10,000 cycles. Two replicate specimens were tested at each strain amplitude. Data acquired during testing (i.e. load and LVDT readings with time) was analyzed using MATLAB and the Alpha-F software developed at NCSU for analyzing fatigue data using the simplified viscoelastic continuum damage approach (S-VECD)(14, 15). The data was post processed using MATLAB to meet the input requirements of the Alpha-F software. This data combined with dynamic modulus and phase angle data obtained previously was used to determine the damage characteristic curve for each mixture. Damage analysis for each mixture was performed using stress and strain history data. Damage parameters (C* and S) were obtained using subroutines within the software and fatigue performance predictions were made using the models available within the Alpha-F software. RESULTS AND DISCUSSION This section presents binder testing performed on the extracted and recovered binder from each mixture. Additionally, the results of the complex modulus testing with the Hirsch model comparison, the TSRST tests, and the fatigue tests, are presented within this section. Recovered Binder Test Results Asphalt Grades, Creep Stiffness and Slope The PG grades were determined for the recovered binder from the four HMA mixes and are summarized in Table 8. The addition of RAP and RAS cause a change in both the high and low PG grades from the virgin PG 64-28 binder that was used. The continuous high and low PG temperatures are greater for the RAS mixtures, although the normal ground shingle mixture is not quite high enough to cause an increase in the high PG grade above the RAP mixture. The increase in temperature on the low side is not significant enough to cause a difference in the low PG grade between the RAP and RAS mixtures. Table 8: Asphalt Grades for Recovered Binder from HMA Mixes Mixture PG Grade Continuous PG Grade RAP Only 70 – 22 71.0 – 26.5 Normal Ground Shingles 70 – 22 75.3 – 25.7 +50 Mesh Shingles -50 Mesh Shingles 76 – 22 76 – 22 77.1 – 25.4 76.3 – 25.7 G*/sinδ values measured using recovered binder from each mixture are presented in Table 9. The G*/sinδ values indicate that the binder extracted from the normal ground shingles mix was stiffer than that which was extracted from the RAP, +50 mesh shingle, or -50 mesh shingle mix, which were comparable to each other. However, the G*sinδ values indicate that at 19 °C, the extracted binder from all four mixes are comparable, and at 16 °C the RAP mixture is stiffer. Creep stiffness and m-values measured using the recovered binder from each mixture are given in Table 10. The creep stiffness values show that those containing RAS were comparable to the mix that contained RAP only at -12 °C, and were less stiff at -18 °C. The RAS mixtures generally have lower m-values than the RAP mixture; so the low temperature PG grade of the RAP mixture would tend to be limited by the S value whereas the m-value would tend to control the low PG grade of the RAS mixtures. Table 9: G*/sinδ Values for Recovered Binder from Mixtures Mixture Temp G*/sinδ Temp G*sinδ (°C) (kPa) (°C) (kPa) RAP Only 70 2.48 19 4831 76 1.21 16 9271 Normal Ground 70 4.20 19 4637 Shingles 76 2.03 16 6363 +50 Mesh Shingles 76 2.47 19 4873 82 1.3 16 6730 -50 Mesh Shingles 76 2.28 19 4473 82 1.2 16 6567 Table 10: Creep Stiffness and m-Values at 60 s for Recovered Binder from Mixtures Temperature S Mixture (°C) (MPa) m-value RAP Only -12 °C 117 0.332 -18 °C 259 0.29 -24 °C ----Normal Ground Shingles -12 °C 118 0.333 -18 °C 244 0.281 -24 °C 478 0.239 +50 Mesh Shingles -12 °C 117 0.322 -18 °C 246 0.284 -24 °C 455 0.256 -50 Mesh Shingles -12 °C 121 0.328 -18 °C 248 0.284 -24 °C 452 0.223 Critical Cracking Temperature The critical cracking temperature was determined for the recovered binder from each of the HMA mixes as well as for the virgin binder, as shown in Figure 1. The addition of recycled materials increases the critical cracking temperature, with the RAP only mixture showing the largest increase. The + 50 mesh and -50 mesh mixtures are similar, with the normal ground shingles showing a higher value. -30 Temperature (°C) -25 -20 -15 -10 -5 0 RAP Only mix Normal +50 Mesh -50 Mesh Virgin Binder Ground Shingles mix Shingles mix Shingles mix Figure 1: Critical Cracking Temperatures for Recovered and Virgin Binders Binder Modulus and Phase Angle This section provides a summary of the binder shear modulus and binder phase angle data measured on recovered binder from the four HMA mixes. Figure 2 shows the comparison of all |G*| master curves and Figure 3 shows the comparison of all binder phase angle (δb) master curves. The recovered binders from the mixes containing RAS are stiffer than the RAP mix and the virgin binder at low reduced frequencies (high temperature). The RAS mixes are nearly indistinguishable from each other. At the higher frequencies (lower temperatures), all of the recovered binder from the HMA mixes have similar values for |G*|, which are stiffer than the virgin binder. The recovered binder phase angle master curves for the RAS mixes are similar and less viscous than the virgin binder and the recovered RAP mix binder. The slope of the RAS mix binder curves match the slope of the virgin binder phase angle master curve, but the recovered RAP mix binder has a steeper slope. |G*| (Pa) 1.E+08 1.E+07 RAP Only 1.E+06 Normal Ground Shingles 1.E+05 +50 Mesh Shingles 1.E+04 -50 Mesh Shingles 1.E+03 Virgin Binder 1.E+02 1.E-04 1.E-02 1.E+00 1.E+02 1.E+04 Reduced Frequency (Hz) Figure 2: Binder Modulus Master Curves for Recovered and Virgin Binders 80 RAP Only 70 Normal Ground Shingles δb (degrees) 60 50 +50 Mesh Shingles 40 -50 Mesh Shingles 30 Virgin Binder 20 1.E-04 1.E-02 1.E+00 1.E+02 1.E+04 Reduced Frequency (Hz) Figure 3: Binder Phase Angle Master Curves for Recovered and Virgin Binders Mixture Test Results Dynamic Modulus and Phase Angle This section provides a summary of the dynamic modulus and phase angle data measured for the four mixtures. Figures 4 and 5 show the comparison of the average dynamic modulus and phase angle master curves for each mixture, respectively. 40000 35000 RAP Only |E*| (MPa) 30000 Normal Ground Shingles 25000 20000 +50 Mesh Shingles 15000 -50 Mesh Shingles 10000 5000 0 1.E-01 1.E+01 1.E+03 1.E+05 1.E+07 1.E+09 Reduced Frequency (Hz) Figure 4: Average Dynamic Modulus Master Curve Comparison of all Mixes 45 40 RAP Only δ(degrees) 35 30 Normal Ground Shingles 25 20 +50 Mesh Shingles 15 -50 Mesh Shingles 10 5 0 1.E-01 1.E+01 1.E+03 1.E+05 1.E+07 1.E+09 Reduced Frequency (Hz) Figure 5: Average Phase Angle Master Curve Comparison of all HMA Mixes From Figure 4, it is clear that the RAP only mixture has a higher mean dynamic modulus than the RAS mixtures at the higher reduced frequencies (i.e. at some test temperatures). It also appears that the RAS mixtures are all similar. The dynamic modulus values at specific frequencies along the master curve were compared using the t-test to determine if there is a significant difference between mixtures. The analysis showed that the RAP mix is significantly different than + 50 mesh and -50 mesh mixes, but not different than the normal ground shingles mixture. The normal ground shingles mix was significantly different than the -50 mesh and RAP mixtures only at higher reduced frequencies (>1x105 Hz). Similarly, the t-test was conducted using phase angle mastercurve data. Over most of the reduced frequency range, the mean values of phase angles were statistically comparable. However, the normal ground shingles values were significantly different than the -50 mesh mix at frequencies greater than 1x109Hz. The RAP mixture has a higher percent binder replacement (Table 6) and a lower asphalt content than the RAS mixtures, which could explain the stiffer dynamic modulus. This may also be an indication of the amount of blending occurring between the recycled and virgin binder in each mix; if the RAP binder blends more than the RAS binder (i.e. the RAS is acting more like a black rock), the RAP mixture would have a stiffer effective binder modulus, resulting in a stiffer measured dynamic modulus for the mixture. Hirsch Model Comparison of Dynamic Modulus The forward calculations of the dynamic modulus from the recovered and virgin binders using the Hirsch model are compared to the measured mixture dynamic modulus values to evaluate the degree of blending that occurred within the HMA mixing procedure. All master curves were shifted to 20 °C. Figures 6 - 9 show the results of these comparisons. The process of recovering binder from the mixture results in full blending of the virgin and recycled binders, so it was expected that this master curve would represent the stiffest possible dynamic modulus values. The virgin binder modulus was used to represent the case where no blending occurs, providing the lower bound dynamic modulus curve. However, for all four mixtures, the measured mixture master curves are stiffer than the predicted master curves from the recovered (fully blended) binder. This phenomenon is not completely understood at this time and is likely due to some other mixture properties. This has been noted by other researchers (16) and will be investigated in the future. |E*| (MPa) 40000 35000 Recovered Binder (Fully Blended) 30000 Measured (Partially Blended) 25000 Virgin Binder (No Blending) 20000 15000 10000 5000 0 1.E-04 1.E-02 1.E+00 1.E+02 1.E+04 1.E+06 1.E+08 Reduced Frequency (Hz) Figure 6: Master Curve Comparison for HMA Mix Containing RAP Only 40000 35000 |E*| (MPa) 30000 25000 Recovered Binder (Full Blending) Measured (Partially Blended) Virgin Binder (No Blending) 20000 15000 10000 5000 0 1.E-04 1.E-01 1.E+02 1.E+05 1.E+08 Reduced Frequency (Hz) Figure 7: Master Curve Comparison for HMA Mix Containing Normal Ground Shingles |E*| (Mpa) 40000 35000 Recovered Binder (Full Blending) 30000 Measured (Partially Blended) 25000 Virgin Binder (No Blending) 20000 15000 10000 5000 0 1.E-04 1.E-01 1.E+02 1.E+05 1.E+08 Reduced Frequency (Hz) Figure 8: Master Curve Comparison for HMA Mix Containing +50 Mesh Shingles |E*| (Mpa) 40000 35000 Recovered Binder (Full Blending) 30000 Measured (Partial Blending) 25000 Virgin Binder (No Blending) 20000 15000 10000 5000 0 1.E-04 1.E-01 1.E+02 1.E+05 1.E+08 Reduced Frequency (Hz) Figure 9: Master Curve Comparison for HMA Mix Containing -50 Mesh Shingles Effective PG Determination To complete the determination of the effective PG grade for each mixture, the binder shear modulus was back calculated using the Hirsch model and the measured mixture the dynamic modulus curves. The back calculated (from mix) and measured (from recovered binder) |G*| master curves are shown in Figure 10. All master curves are shifted to 20 °C. 1.E+09 RAP Only 1.E+08 RAP Only Hirsch |G*| (Pa) 1.E+07 Normal Ground Shingles 1.E+06 Normal Ground Shingles - Hirsch 1.E+05 +50 Mesh Shingles 1.E+04 +50 Mesh Shingles - Hirsch 1.E+03 -50 Mesh Shingles 1.E+02 1.E-04 1.E-02 1.E+00 1.E+02 Reduced Frequency (Hz) 1.E+04 -50 Mesh Shingles - Hirsch Virgin Binder Figure 10: Master Curve Comparison of Back Calculated |G*| from the |E*| of the Mix and Measured |G*| for Recovered Binder The effective high PG temperature for each mixture determined using the back calculated |G*| (partial blending) and the measured |G*| (full blending) curves are summarized in Table 11. Using the recovered binder analysis, the RAS mixtures all have similar high PG temperatures that are greater than that for the RAP mixture. The RAP mixture shows a high PG temperature below the virgin binder grade, which is likely an artifact of extrapolating the shift factors. The effective high PG temperatures based on the back calculated values are greater than those for the measured values, as expected. However, the trend among the mixtures is different. The normal ground shingles have the highest value, and the RAP and +50 mesh mixtures are more similar. Table 11: Comparison of Effective PG for HMA Mixes from Measured Extracted (Fully Blended) |G*| and Back Calculated |G*| High PG High PG Mixture Temperature: Temperature:Back Measured |G*| Calculated |G*| RAP Only 61.5 88.0 Normal Ground Shingles +50 Mesh Shingles -50 Mesh Shingles 78.5 93.0 76.0 80.0 74.4 77.1 Thermal Stress Restrained Specimen Tensile Strength Test The average temperature and load at failure in the TSRST test for each mix are shown in Figures 11 and 12, respectively. Standard t-tests indicate that the mean values for load and temperature at failure are not significantly different for any of the four mixes. The standard deviations for each are represented as error bars. -31 Temperature at Failure (°C) -30 -29 -28 -27 -26 -25 -24 -23 -22 -21 -20 RAP Only Normal Ground Shingles +50 Mesh Shingles -50 Mesh Shingles Figure 11: Comparison of Average Temperature at Failure for Each Mix 1600 1400 Load at Failure (kg) 1200 1000 800 600 400 200 0 RAP Only Normal Ground Shingles +50 Mesh Shingles -50 Mesh Shingles Figure 12: Comparison of the Average Load at Failure for Each Mix Fatigue Testing Figures 13a and 13b presents damage characteristic curves obtained for the RAP only and +50 mesh shingles mixtures, respectively. Predicted fatigue life of the two mixtures at 200C and -200C are presented in Figure 14. Fatigue curves at 20 0C indicate that the +50 mesh shingles mixture performs better than the RAP mix. At lower temperatures (-20 0C), the difference in fatigue life between mixtures is negligible, especially at higher strain levels. Also, the slope of the curve for the RAP mixture is steeper than that for the +50 mesh shingles mix. The endurance limit values for +50 mesh shingles mixtures at 200C and -200C were found to be 93 microstrain and 15 microstrain, respectively. These values are 40% and 20% higher than the corresponding values for the RAP mixture. It should be recognized, however, that the improvement in fatigue performance is likely due in part to the higher total binder content of the +50 mesh shingles mix, and not just a result of the shingles alone. Also, fibers that could have been present in +50 mesh shingles may result in increased fatigue resistance when compared to the RAP only mixture. 1.00 R57F1c R57F1d C* 0.75 R57F3b R57F3a 0.50 0.25 0.00 0.0E+00 2.0E+05 4.0E+05 Damage Parameter 6.0E+05 (a) 1.00 G60F1d G60F2a G60F2b G60F3a G60F3b C* 0.75 0.50 0.25 0.00 0.0E+00 2.0E+05 4.0E+05 Damage Parameter 6.0E+05 (b) Figure 13: Damage Characteristic Curves for RAP and +50 mesh Shingles Mixtures Strain Amplitude (10-6) 10000 +50 mesh shingles mix, 20 C +50 mesh shingles mix, -20 C RAP mix, 20 C RAP mix, -20 C 1000 100 10 1.0E-01 1.0E+03 1.0E+07 1.0E+11 1.0E+15 Number of Cycles Figure 14: Comparison of the Fatigue Curves for RAP and +50 mesh Shingles Mixtures SUMMARY AND CONCLUSIONS This study compared the use of RAP and RAS as a recycled aggregate and binder source in HMA pavement. One RAP and three RAS mixtures were evaluated based on the PG grade, DSR, creep stiffness and slope values, critical cracking temperature, and |G*| and δb master curves of extracted binder from each mix. The potential performance of the mixtures were also evaluated by developing the |E*| and δ master curves, the comparison of the back calculated |G*| values as determined by the Hirsch model and the effective high temperature PG grade of the mix. The mixes were also evaluated for low temperature and fatigue performance. Conclusions based on the results of the laboratory tests performed in this study are: Recovered Binder Testing The continuous PG grade shows that RAS mixtures are stiffer at the high temperature end, and that RAP and RAS have comparable stiffness at the low temperature end. This is expected because the RAS binder is much stiffer than the RAP binder. Creep stiffness and m-value trends with temperature for the recovered binders show that the low PG grade of the RAP tends to be controlled by the S values while the m-value controls the low PG grade of the RAS mixtures. Critical cracking temperatures for the recovered RAS mixture binder were lower than the RAP mixture binder, indicating that the RAS mixtures would have better low temperature performance. |G*| master curves for the three recovered RAS mixture binders were very similar. The recovered binder from the RAP mixture was softer than the RAS mixtures at low reduced frequencies, but was comparable to the RAS mixture binders at the higher reduced frequencies. The recovered binder from the RAP mixture had a higher phase angle and steeper rate of change than the RAS mixture binders. The effective high temperature PG grade for the mixtures determined from the measured |G*| values on recovered binders show that RAP has the lowest value, and that the RAS mixes are very similar to each other. Mixture Testing |E*| master curves for the three RAS mixtures are statistically the same over most of the reduced frequency range. The RAP mix shows a stiffer average response, but is only statistically different than the +50 and -50 mesh RAS mixtures. The phase angle curves for all mixtures were statistically similar. The effective high temperature PG grade for the mixtures determined using the back calculated |G*| values (from measured mix |E*|) show the +50 and -50 mesh mixtures to have comparable effective PG grades, which were lower than the effective PG grades for RAP and Normal Ground Shingle mixes. TSRST tests showed that the load and temperature at failure for the four mixtures were not significantly different, indicating similar low temperature performance. Fatigue tests and subsequent evaluation using S-VECD analysis indicated that +50 mesh shingles mixture performs better and has a higher fatigue endurance limit than the RAP mixture. The difference in performance decreases as the temperature decreases, which correlates with the TSRST results. The improvement in fatigue performance is likely due in part to the higher total binder content and possible presence of fibers in the +50 mesh shingles mixture. The comparison of the RAS and RAP mixtures is different based on the recovered binder and mixture testing. The binder testing indicates that the RAS mixtures are stiffer than the RAP mix at high temperatures and would perform better with respect to low temperature cracking. The mixture testing shows that the RAP mix has a stiffer response than the RAS mixtures; this is likely due to a combination of effects that include binder content, source material properties, and blending. The stiffer RAP mixture response causes the RAP mixture to have a lower predicted laboratory fatigue life than the RAS mixtures; however the relative performance of these mixtures in the field will also depend on the pavement structure. The low temperature evaluation of these mixtures indicates the RAP and RAS mixtures will have similar performance. As agencies make the decision whether to use RAS or RAP in a mixture, the performance as well as the cost of the materials and amounts of virgin materials required (RAS mixtures require more virgin ac) need to be considered. RECCOMMENDATIONS FOR FUTURE WORK Future research should be performed with plant produced mixtures, as plant mixes tend to differ slightly from lab mixes in their physical and mechanical properties. Additionally, testing should include mixtures that contain higher RAS and RAP percentages. Long term field performance of RAS mixtures also needs to be evaluated. ACKNOWLEDGEMENTS The authors would like to acknowledge Pike Industries, Inc., ERRCO, and RASTech, Inc. for their donations of materials for this project. The New Hampshire Industrial Research Council and RASTech, Inc. provided funding for this project and the NHDOT provided valuable research direction and support. Applied Asphalt Technologies performed all the binder testing for this study. Additionally, special thanks are extended to Marcelo Medeiros, Katie Gray and Kelly Barry for their assistance with specimen preparation and laboratory testing performed at UNH. REFERENCES 1. J. S. Daniel, W. S. Mogawer. “Determining the Effective PG Grade of Binder in RAP Mixes” Final Research Report to The New England Transportation Consortium, 2010. 2. K. W. Lee, A. Shukla, S. Vankatram, N. Soupharath. “Evaluation of Permanent Deformation and Fatigue Cracking Resistance Characteristics of Recycled Pavement Binder” Final Research Report to Rhode Island DOT, 1998. 3. R. McDaniel, R. M. Anderson. “Recommended Use of Reclaimed Asphalt Pavement in the Superpave Mix Design Method: Technician’s Manual”, NCHRP Report 452, Transportation Research Board- National Research Council, National Academy Press, Washington, D.C., 2001. 4. R. McDaniel, R. M. Anderson. “Recommended Use of Reclaimed Asphalt Pavement in the Superpave Mix Design Method: Guidelines”. NCHRP Research Results Digest, Number 253, 2001. 5. R. S. McDaniel, H. Soleymani, R.M. Anderson, P. Turner, R. Peterson. “Recommended Use of Reclaimed Asphalt Pavement in the Superpave Mix Design Method”. Contractor’s Final Report, NCHRP Web Document 30 (Project D9-12), 2000. 6. H. Soleymani, M. Anderson, R. McDaniel, M. Abdelrahman. “Investigation of the Black Rock Issue for Recycled Asphalt Mixtures”, Journal of the Association of Asphalt Paving Technologists, Vol. 69, p. 366-390, 2000. 7. J. Stephens, J. Mahoney, C. Dippold. “Determination of the PG Binder Grade to Use in a RAP Mix”, Final Report JHR 00-278, Project 99-1, Connecticut Department of Transportation, 2001. 8. M. Stroup-Gardiner, C. Wagner. “Use of Reclaimed Asphalt Pavement in Superpave Hot-Mix Asphalt Applications”, Transportation Research Record 1681, 1999. 9. “NHDOT Construction Manual: Division 400 – Pavements”, New Hampshire Department of Transportation. April 2009. 10. D. W. Christensen., T. Pellinen, R. Bonaquist. “Hirsch Model for Estimating the Modulus of Asphalt Concrete”, Journal of the Association of Asphalt Paving Technologists, Vol. 72, pp. 97 – 121, 2003. 11. D. W. Christensen, D. A. Anderson. “Interpretation of Dynamic Mechanical Test Data for Paving Grade Asphalts”, Journal of the Association of Asphalt Paving Technologists, Vol. 61, pp. 67 – 98, 1992. 12. AASHTO Provisional Standards, American Association of State Highway and Transportation Officials, Washington, D.C 13. Proposed standard for Determining the Damage Characteristic Curve of Asphalt Concrete from Direct Tension Cyclic Fatigue Tests. TP XX-XX. 14. Underwood, B.S., Y.R. Kim, M.N. Guddati. “Improved Calculation Method of Damage Parameter in Viscoelastic Continuum Damage Model,” International Journal of Pavement Engineering. 2010. In Press. 15. Y. R. Kim, M. N. Guddati, B. S. Underwood, T. Y. Yun, V. Subramanian, S. Savadatti, S. Thirunavukkarasu.. “Development of a Multiaxial VEPCD-FEP++.” Final Report FHWA-HRT-08-073. Federal Highway Administration, 2008. 16. A. R. Copeland, J. A. D’Angelo, R. N. Dongre, G. A. Sholar. “Field Evalueation of High Reclaimed Asphalt Pavement-Warm_mix Asphalt Project in Florida: Case Study. Transportation Research Board Annual Meeting 2010, paper #10-3792.